#------------------------------------------------------------------------------
#$Date: 2016-03-26 19:24:35 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180433 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/02/7210225.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7210225
loop_
_publ_author_name
'Kastner, Katharina'
'Streb, Carsten'
_publ_section_title
;
 Solvent-shielding allows the self-assembly of supramolecular 1D barium
 vanadate chains
;
_journal_issue                   24
_journal_name_full               CrystEngComm
_journal_page_first              4948
_journal_paper_doi               10.1039/c3ce40536b
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C24 H54 Ba2 N8 O36 V10'
_chemical_formula_weight         1814.83
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                104.74(3)
_cell_angle_beta                 103.04(3)
_cell_angle_gamma                107.93(3)
_cell_formula_units_Z            1
_cell_length_a                   11.340(2)
_cell_length_b                   11.638(2)
_cell_length_c                   12.492(3)
_cell_measurement_reflns_used    368
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      23.1
_cell_measurement_theta_min      6.7
_cell_volume                     1431.8(7)
_computing_cell_refinement       SUPERGUI
_computing_data_collection       SUPERGUI
_computing_data_reduction        SUPERGUI
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    SHELXS-97
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Nonius-Kappa CCD'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1061
_diffrn_reflns_av_sigmaI/netI    0.0638
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            34583
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         5.82
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    2.999
_exptl_absorpt_correction_T_max  0.931
_exptl_absorpt_correction_T_min  0.741
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow-orange
_exptl_crystal_density_diffrn    2.105
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             884
_exptl_crystal_size_max          0.09
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.118
_refine_diff_density_min         -1.157
_refine_diff_density_rms         0.154
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     436
_refine_ls_number_reflns         5789
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.030
_refine_ls_R_factor_all          0.0770
_refine_ls_R_factor_gt           0.0503
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0578P)²+5.4115P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1138
_refine_ls_wR_factor_ref         0.1261
_reflns_number_gt                4323
_reflns_number_total             5789
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            c3ce40536b.txt
_cod_data_source_block           p-1a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'multiscan' changed to
'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        1431.8(5)
_cod_database_code               7210225
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.9191(13) 0.5939(13) 0.2155(12) 0.048(4) Uani 0.587(14) 1 d P A 1
H1 H 1.0015 0.6108 0.2658 0.057 Uiso 0.587(14) 1 calc PR A 1
C2 C 0.9339(16) 0.4045(15) 0.0916(13) 0.053(4) Uani 0.587(14) 1 d P A 1
H2A H 0.8812 0.3375 0.0173 0.080 Uiso 0.587(14) 1 calc PR A 1
H2B H 0.9454 0.3670 0.1514 0.080 Uiso 0.587(14) 1 calc PR A 1
H2C H 1.0181 0.4509 0.0878 0.080 Uiso 0.587(14) 1 calc PR A 1
C3 C 0.736(2) 0.458(3) 0.038(2) 0.099(9) Uani 0.587(14) 1 d P A 1
H3A H 0.7153 0.3827 -0.0282 0.148 Uiso 0.587(14) 1 calc PR A 1
H3B H 0.7347 0.5282 0.0106 0.148 Uiso 0.587(14) 1 calc PR A 1
H3C H 0.6725 0.4412 0.0768 0.148 Uiso 0.587(14) 1 calc PR A 1
N1 N 0.8682(11) 0.4933(10) 0.1198(10) 0.045(3) Uani 0.587(14) 1 d P A 1
C4 C 0.854(4) 0.567(3) 0.026(3) 0.099(13) Uani 0.413(14) 1 d P A 2
H4A H 0.8288 0.5097 -0.0533 0.148 Uiso 0.413(14) 1 calc PR A 2
H4B H 0.9158 0.5482 0.0771 0.148 Uiso 0.413(14) 1 calc PR A 2
H4C H 0.8928 0.6545 0.0295 0.148 Uiso 0.413(14) 1 calc PR A 2
C5 C 0.610(4) 0.460(3) -0.025(2) 0.116(15) Uani 0.413(14) 1 d P A 2
H5A H 0.6256 0.4207 -0.0951 0.174 Uiso 0.413(14) 1 calc PR A 2
H5B H 0.5544 0.5054 -0.0423 0.174 Uiso 0.413(14) 1 calc PR A 2
H5C H 0.5681 0.3950 0.0034 0.174 Uiso 0.413(14) 1 calc PR A 2
C6 C 0.746(3) 0.619(2) 0.1696(19) 0.060(7) Uani 0.413(14) 1 d P A 2
H6 H 0.6711 0.6227 0.1870 0.072 Uiso 0.413(14) 1 calc PR A 2
N1A N 0.733(3) 0.5497(19) 0.0630(15) 0.072(7) Uani 0.413(14) 1 d P A 2
C8 C 0.6562(19) 0.977(2) 0.0468(16) 0.086(7) Uani 0.613(14) 1 d P B 1
H8A H 0.5704 0.9483 -0.0090 0.129 Uiso 0.613(14) 1 calc PR B 1
H8B H 0.6605 0.9111 0.0795 0.129 Uiso 0.613(14) 1 calc PR B 1
H8C H 0.7208 0.9925 0.0084 0.129 Uiso 0.613(14) 1 calc PR B 1
C9 C 0.579(2) 1.147(3) 0.140(3) 0.128(12) Uani 0.613(14) 1 d P B 1
H9A H 0.5054 1.0922 0.0699 0.192 Uiso 0.613(14) 1 calc PR B 1
H9B H 0.6092 1.2332 0.1395 0.192 Uiso 0.613(14) 1 calc PR B 1
H9C H 0.5516 1.1458 0.2073 0.192 Uiso 0.613(14) 1 calc PR B 1
N2 N 0.6832(13) 1.1000(17) 0.1444(15) 0.075(5) Uani 0.613(14) 1 d P B 1
C10 C 0.6747(19) 1.246(2) 0.126(2) 0.046(6) Uani 0.387(14) 1 d P B 2
H10A H 0.6825 1.3146 0.0954 0.069 Uiso 0.387(14) 1 calc PR B 2
H10B H 0.6262 1.2515 0.1795 0.069 Uiso 0.387(14) 1 calc PR B 2
H10C H 0.6295 1.1645 0.0625 0.069 Uiso 0.387(14) 1 calc PR B 2
C11 C 0.9175(18) 1.3594(18) 0.1876(19) 0.037(5) Uani 0.387(14) 1 d P B 2
H11A H 0.8875 1.4111 0.1482 0.056 Uiso 0.387(14) 1 calc PR B 2
H11B H 0.9679 1.3231 0.1479 0.056 Uiso 0.387(14) 1 calc PR B 2
H11C H 0.9714 1.4122 0.2671 0.056 Uiso 0.387(14) 1 calc PR B 2
N2A N 0.8047(14) 1.2559(13) 0.1869(12) 0.027(4) Uani 0.387(14) 1 d P B 2
C7 C 0.8023(12) 1.1573(10) 0.2347(9) 0.064(3) Uani 1 1 d . . .
C12 C 0.8980(13) 0.8370(13) -0.0109(11) 0.044(4) Uani 0.62(2) 1 d P A 1
H12 H 0.9829 0.8567 -0.0138 0.053 Uiso 0.62(2) 1 calc PR A 1
C12A C 0.751(2) 0.815(2) 0.006(2) 0.053(7) Uani 0.38(2) 1 d P A 2
H12A H 0.6710 0.8078 0.0171 0.063 Uiso 0.38(2) 1 calc PR A 2
C13 C 1.1336(6) 1.2775(7) 0.5010(6) 0.0316(15) Uani 1 1 d . . .
H13 H 1.0488 1.2690 0.4991 0.038 Uiso 1 1 calc R . .
C14 C 1.1840(9) 1.5070(8) 0.5598(9) 0.052(2) Uani 1 1 d . . .
H14A H 1.2582 1.5843 0.5762 0.078 Uiso 1 1 calc R . .
H14B H 1.1580 1.5112 0.6282 0.078 Uiso 1 1 calc R . .
H14C H 1.1124 1.4986 0.4961 0.078 Uiso 1 1 calc R . .
C15 C 1.3562(8) 1.4195(8) 0.5355(8) 0.047(2) Uani 1 1 d . . .
H15A H 1.4036 1.5102 0.5555 0.071 Uiso 1 1 calc R . .
H15B H 1.3596 1.3734 0.4614 0.071 Uiso 1 1 calc R . .
H15C H 1.3952 1.3912 0.5949 0.071 Uiso 1 1 calc R . .
C16 C 0.651(2) 0.7020(18) -0.154(2) 0.165(10) Uani 1 1 d . A .
H16A H 0.6213 0.6941 -0.0892 0.248 Uiso 1 1 calc R . .
H16B H 0.6367 0.6182 -0.2048 0.248 Uiso 1 1 calc R . .
H16C H 0.6027 0.7401 -0.1972 0.248 Uiso 1 1 calc R . .
C17 C 0.8375(15) 0.7986(15) -0.1975(19) 0.127(7) Uani 1 1 d . A .
H17A H 0.9292 0.8530 -0.1625 0.190 Uiso 1 1 calc R . .
H17B H 0.7927 0.8386 -0.2411 0.190 Uiso 1 1 calc R . .
H17C H 0.8271 0.7168 -0.2492 0.190 Uiso 1 1 calc R . .
N4 N 1.2200(5) 1.3946(5) 0.5274(5) 0.0298(12) Uani 1 1 d . . .
N5 N 0.7861(14) 0.7808(8) -0.1121(6) 0.092(4) Uani 1 1 d . . .
O2 O 1.1197(4) 0.9196(4) 0.5099(4) 0.0237(9) Uani 1 1 d . . .
O3 O 1.3543(4) 1.0969(4) 0.5156(3) 0.0196(8) Uani 1 1 d . . .
O4 O 1.3745(4) 0.9367(4) 0.6093(3) 0.0214(9) Uani 1 1 d . A .
O5 O 1.1986(4) 0.7321(4) 0.4149(4) 0.0260(9) Uani 1 1 d . A .
O6 O 1.4112(4) 0.9064(4) 0.4060(3) 0.0190(8) Uani 1 1 d . . .
O7 O 1.4313(4) 0.7329(4) 0.5046(4) 0.0258(9) Uani 1 1 d . . .
O8 O 1.3876(4) 1.0724(4) 0.3007(4) 0.0250(9) Uani 1 1 d . . .
O9 O 0.6728(4) 0.8635(5) 0.2596(4) 0.0315(11) Uani 1 1 d . . .
O10 O 1.4361(4) 0.8773(4) 0.1913(4) 0.0271(10) Uani 1 1 d . . .
O11 O 1.1754(4) 0.9088(4) 0.3148(4) 0.0213(9) Uani 1 1 d . A .
O12 O 1.2502(5) 0.5258(4) 0.3002(4) 0.0361(11) Uani 1 1 d . . .
O13 O 1.4617(4) 0.7058(4) 0.2946(4) 0.0283(10) Uani 1 1 d . . .
O14 O 1.1554(4) 1.1773(4) 0.4786(5) 0.0392(12) Uani 1 1 d . . .
O15 O 1.2270(4) 0.7099(4) 0.2068(4) 0.0278(10) Uani 1 1 d . . .
O16 O 1.1905(5) 0.8749(5) 0.0958(4) 0.0332(11) Uani 1 1 d . . .
O18 O 0.8562(7) 0.6798(6) 0.2482(6) 0.0636(18) Uani 1 1 d . . .
O19 O 0.9014(8) 1.1366(8) 0.2641(6) 0.076(2) Uani 1 1 d . A .
O26 O 0.8735(9) 0.8584(11) 0.0835(5) 0.127(4) Uani 1 1 d . . .
V3 V 1.27362(10) 0.87686(11) 0.21958(9) 0.0240(2) Uani 1 1 d . . .
V4 V 1.44687(10) 1.12604(10) 0.69290(9) 0.0234(2) Uani 1 1 d . . .
V5 V 1.50804(10) 0.89475(9) 0.56613(9) 0.0199(2) Uani 1 1 d . . .
V6 V 1.31484(10) 0.67950(10) 0.33349(10) 0.0261(3) Uani 1 1 d . . .
V10 V 1.23513(10) 0.89569(10) 0.45971(9) 0.0201(2) Uani 1 1 d . . .
Ba1 Ba 0.94465(4) 0.93776(4) 0.31392(3) 0.02947(14) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N1 C1 O18 124.1(12) . .
C1 N1 C2 122.4(12) . .
C1 N1 C3 120.9(13) . .
C2 N1 C3 116.6(13) . .
O18 C6 N1A 121(2) . .
O18 C6 Ba1 45.0(8) . .
N1A C6 Ba1 125.5(17) . .
C6 N1A C5 124(3) . .
C6 N1A C4 119(3) . .
C5 N1A C4 116(3) . .
C7 N2 C9 124(2) . .
C7 N2 C8 118.9(11) . .
C9 N2 C8 117.2(19) . .
C7 N2A C10 113.2(14) . .
C7 N2A C11 129.1(13) . .
C10 N2A C11 117.7(14) . .
O19 C7 N2 137.9(11) . .
O19 C7 N2A 119.7(11) . .
N2 C7 N2A 78.0(9) . .
O26 C12 N5 114.3(12) . .
O26 C12A N5 98.1(15) . .
O14 C13 N4 125.7(6) . .
C13 N4 C15 121.8(6) . .
C13 N4 C14 120.4(6) . .
C15 N4 C14 117.5(6) . .
C17 N5 C12 102.8(14) . .
C17 N5 C16 114.1(14) . .
C12 N5 C16 142.3(15) . .
C17 N5 C12A 159.3(14) . .
C12 N5 C12A 67.6(11) . .
C16 N5 C12A 79.6(15) . .
V10 O2 Ba1 147.8(2) . 2_776
V10 O2 Ba1 103.16(19) . .
Ba1 O2 Ba1 97.36(12) 2_776 .
V5 O3 V4 107.36(17) 2_876 .
V5 O3 V10 104.78(17) 2_876 .
V4 O3 V10 98.12(17) . .
V5 O4 V4 107.6(2) . .
V5 O4 V10 105.8(2) . .
V4 O4 V10 107.89(19) . .
V10 O5 V6 113.7(2) . .
V5 O6 V5 103.24(17) 2_876 .
V5 O6 V10 99.73(16) 2_876 .
V5 O6 V10 90.66(16) . .
V5 O6 V4 89.76(16) 2_876 2_876
V5 O6 V4 98.60(15) . 2_876
V10 O6 V4 164.92(19) . 2_876
V5 O6 V6 168.0(2) 2_876 .
V5 O6 V6 87.41(15) . .
V10 O6 V6 85.43(14) . .
V4 O6 V6 83.14(13) 2_876 .
V5 O6 V3 87.96(15) 2_876 .
V5 O6 V3 168.5(2) . .
V10 O6 V3 84.60(13) . .
V4 O6 V3 84.05(13) 2_876 .
V6 O6 V3 81.74(13) . .
V5 O7 V6 110.8(2) . .
V5 O8 V3 111.7(2) 2_876 .
V4 O9 Ba1 146.4(2) 2_776 .
V4 O10 V3 115.2(2) 2_876 .
V10 O11 V3 113.5(2) . .
V10 O11 Ba1 102.83(17) . .
V3 O11 Ba1 142.9(2) . .
V6 O13 V4 115.4(2) . 2_876
C13 O14 Ba1 118.8(4) . .
V3 O15 V6 115.6(2) . .
C6 O18 C1 99.5(12) . .
C6 O18 Ba1 115.7(10) . .
C1 O18 Ba1 130.5(7) . .
C7 O19 Ba1 132.8(7) . .
C12 O26 C12A 79.8(12) . .
C12 O26 Ba1 152.4(9) . .
C12A O26 Ba1 127.8(11) . .
O16 V3 O15 105.2(2) . .
O16 V3 O11 103.2(2) . .
O15 V3 O11 93.9(2) . .
O16 V3 O10 101.1(2) . .
O15 V3 O10 89.6(2) . .
O11 V3 O10 153.53(18) . .
O16 V3 O8 100.4(2) . .
O15 V3 O8 154.05(18) . .
O11 V3 O8 84.50(18) . .
O10 V3 O8 81.07(18) . .
O16 V3 O6 173.0(2) . .
O15 V3 O6 81.60(17) . .
O11 V3 O6 77.57(16) . .
O10 V3 O6 77.00(16) . .
O8 V3 O6 72.74(15) . .
O16 V3 V6 137.75(19) . .
O15 V3 V6 32.64(14) . .
O11 V3 V6 87.31(13) . .
O10 V3 V6 81.56(14) . .
O8 V3 V6 121.51(12) . .
O6 V3 V6 48.99(10) . .
O16 V3 V10 136.08(17) . .
O15 V3 V10 80.36(15) . .
O11 V3 V10 33.24(12) . .
O10 V3 V10 122.64(13) . .
O8 V3 V10 84.41(13) . .
O6 V3 V10 45.75(10) . .
V6 V3 V10 60.38(4) . .
O16 V3 V5 130.44(19) . 2_876
O15 V3 V5 124.09(15) . 2_876
O11 V3 V5 80.08(13) . 2_876
O10 V3 V5 76.31(13) . 2_876
O8 V3 V5 30.10(11) . 2_876
O6 V3 V5 42.64(10) . 2_876
V6 V3 V5 91.46(5) . 2_876
V10 V3 V5 64.58(4) . 2_876
O9 V4 O10 106.1(2) 2_776 2_876
O9 V4 O13 103.2(2) 2_776 2_876
O10 V4 O13 96.5(2) 2_876 2_876
O9 V4 O4 99.0(2) 2_776 .
O10 V4 O4 94.0(2) 2_876 .
O13 V4 O4 151.64(19) 2_876 .
O9 V4 O3 97.6(2) 2_776 .
O10 V4 O3 155.08(18) 2_876 .
O13 V4 O3 85.41(18) 2_876 .
O4 V4 O3 74.33(16) . .
O9 V4 O6 170.06(19) 2_776 2_876
O10 V4 O6 82.72(17) 2_876 2_876
O13 V4 O6 79.92(17) 2_876 2_876
O4 V4 O6 75.38(16) . 2_876
O3 V4 O6 73.12(14) . 2_876
O9 V4 V6 134.84(18) 2_776 2_876
O10 V4 V6 84.59(16) 2_876 2_876
O13 V4 V6 31.71(13) 2_876 2_876
O4 V4 V6 124.35(13) . 2_876
O3 V4 V6 84.22(13) . 2_876
O6 V4 V6 49.18(10) 2_876 2_876
O9 V4 V5 133.46(18) 2_776 .
O10 V4 V5 78.70(15) 2_876 .
O13 V4 V5 122.55(14) 2_876 .
O4 V4 V5 35.00(12) . .
O3 V4 V5 79.40(11) . .
O6 V4 V5 42.64(10) 2_876 .
V6 V4 V5 91.41(5) 2_876 .
O8 V5 O7 107.1(2) 2_876 .
O8 V5 O4 99.93(19) 2_876 .
O7 V5 O4 100.3(2) . .
O8 V5 O3 94.81(19) 2_876 2_876
O7 V5 O3 93.75(19) . 2_876
O4 V5 O3 155.55(17) . 2_876
O8 V5 O6 87.64(19) 2_876 2_876
O7 V5 O6 164.06(19) . 2_876
O4 V5 O6 82.48(17) . 2_876
O3 V5 O6 78.74(16) 2_876 2_876
O8 V5 O6 164.0(2) 2_876 .
O7 V5 O6 88.03(18) . .
O4 V5 O6 81.87(16) . .
O3 V5 O6 78.72(16) 2_876 .
O6 V5 O6 76.76(17) 2_876 .
O8 V5 V10 138.27(15) 2_876 .
O7 V5 V10 84.82(15) . .
O4 V5 V10 38.39(12) . .
O3 V5 V10 124.82(12) 2_876 .
O6 V5 V10 87.99(11) 2_876 .
O6 V5 V10 46.11(11) . .
O8 V5 V6 145.30(16) 2_876 .
O7 V5 V6 38.50(15) . .
O4 V5 V6 93.29(13) . .
O3 V5 V6 85.35(12) 2_876 .
O6 V5 V6 126.06(11) 2_876 .
O6 V5 V6 49.54(11) . .
V10 V5 V6 60.41(4) . .
O8 V5 V3 38.25(16) 2_876 2_876
O7 V5 V3 145.16(15) . 2_876
O4 V5 V3 92.21(13) . 2_876
O3 V5 V3 87.37(12) 2_876 2_876
O6 V5 V3 49.40(11) 2_876 2_876
O6 V5 V3 126.10(12) . 2_876
V10 V5 V3 122.52(5) . 2_876
V6 V5 V3 172.22(5) . 2_876
O8 V5 V4 84.67(15) 2_876 .
O7 V5 V4 137.69(16) . .
O4 V5 V4 37.43(13) . .
O3 V5 V4 126.34(12) 2_876 .
O6 V5 V4 47.60(11) 2_876 .
O6 V5 V4 87.44(11) . .
V10 V5 V4 62.48(5) . .
V6 V5 V4 122.78(5) . .
V3 V5 V4 60.21(4) 2_876 .
O12 V6 O13 103.8(2) . .
O12 V6 O15 104.6(2) . .
O13 V6 O15 93.7(2) . .
O12 V6 O5 100.3(2) . .
O13 V6 O5 154.7(2) . .
O15 V6 O5 87.45(18) . .
O12 V6 O7 100.2(2) . .
O13 V6 O7 87.51(19) . .
O15 V6 O7 154.05(18) . .
O5 V6 O7 80.76(17) . .
O12 V6 O6 173.0(2) . .
O13 V6 O6 79.60(17) . .
O15 V6 O6 81.03(17) . .
O5 V6 O6 75.63(16) . .
O7 V6 O6 73.70(16) . .
O12 V6 V3 136.38(18) . .
O13 V6 V3 86.30(15) . .
O15 V6 V3 31.78(14) . .
O5 V6 V3 81.48(13) . .
O7 V6 V3 122.83(13) . .
O6 V6 V3 49.28(10) . .
O12 V6 V4 136.47(19) . 2_876
O13 V6 V4 32.91(14) . 2_876
O15 V6 V4 81.30(15) . 2_876
O5 V6 V4 123.19(13) . 2_876
O7 V6 V4 85.94(14) . 2_876
O6 V6 V4 47.68(10) . 2_876
V3 V6 V4 60.75(4) . 2_876
O12 V6 V5 130.81(19) . .
O13 V6 V5 82.31(14) . .
O15 V6 V5 123.87(14) . .
O5 V6 V5 76.16(13) . .
O7 V6 V5 30.66(12) . .
O6 V6 V5 43.05(10) . .
V3 V6 V5 92.25(5) . .
V4 V6 V5 65.59(5) 2_876 .
O12 V6 V10 130.80(19) . .
O13 V6 V10 125.09(15) . .
O15 V6 V10 79.29(14) . .
O5 V6 V10 30.55(13) . .
O7 V6 V10 78.84(12) . .
O6 V6 V10 45.50(10) . .
V3 V6 V10 59.83(4) . .
V4 V6 V10 92.73(5) 2_876 .
V5 V6 V10 59.68(4) . .
O2 V10 O5 107.1(2) . .
O2 V10 O11 97.99(19) . .
O5 V10 O11 98.8(2) . .
O2 V10 O4 100.35(19) . .
O5 V10 O4 94.59(19) . .
O11 V10 O4 153.00(19) . .
O2 V10 O3 94.24(19) . .
O5 V10 O3 157.29(18) . .
O11 V10 O3 85.44(17) . .
O4 V10 O3 73.63(17) . .
O2 V10 O6 168.42(19) . .
O5 V10 O6 84.33(18) . .
O11 V10 O6 81.46(16) . .
O4 V10 O6 76.61(16) . .
O3 V10 O6 74.18(15) . .
O2 V10 V5 135.81(15) . .
O5 V10 V5 79.55(15) . .
O11 V10 V5 124.69(13) . .
O4 V10 V5 35.78(12) . .
O3 V10 V5 79.76(11) . .
O6 V10 V5 43.23(10) . .
O2 V10 V3 131.20(15) . .
O5 V10 V3 85.34(16) . .
O11 V10 V3 33.30(12) . .
O4 V10 V3 126.08(13) . .
O3 V10 V3 86.26(12) . .
O6 V10 V3 49.65(10) . .
V5 V10 V3 92.37(5) . .
O2 V10 V6 142.51(16) . .
O5 V10 V6 35.74(15) . .
O11 V10 V6 86.80(13) . .
O4 V10 V6 90.56(12) . .
O3 V10 V6 123.25(11) . .
O6 V10 V6 49.07(10) . .
V5 V10 V6 59.92(5) . .
V3 V10 V6 59.79(4) . .
O2 V10 Ba1 50.72(14) . .
O5 V10 Ba1 106.87(15) . .
O11 V10 Ba1 47.39(12) . .
O4 V10 Ba1 147.67(12) . .
O3 V10 Ba1 92.45(11) . .
O6 V10 Ba1 128.36(11) . .
V5 V10 Ba1 169.82(4) . .
V3 V10 Ba1 80.49(4) . .
V6 V10 Ba1 120.95(5) . .
O26 Ba1 O18 75.9(3) . .
O26 Ba1 O19 77.0(3) . .
O18 Ba1 O19 144.6(2) . .
O26 Ba1 O11 87.7(3) . .
O18 Ba1 O11 81.27(18) . .
O19 Ba1 O11 119.85(19) . .
O26 Ba1 O2 137.7(3) . 2_776
O18 Ba1 O2 120.82(17) . 2_776
O19 Ba1 O2 68.87(17) . 2_776
O11 Ba1 O2 130.74(12) . 2_776
O26 Ba1 O9 80.4(2) . .
O18 Ba1 O9 76.89(18) . .
O19 Ba1 O9 76.6(2) . .
O11 Ba1 O9 157.09(13) . .
O2 Ba1 O9 68.19(13) 2_776 .
O26 Ba1 O2 139.7(3) . .
O18 Ba1 O2 81.46(18) . .
O19 Ba1 O2 133.6(2) . .
O11 Ba1 O2 55.85(12) . .
O2 Ba1 O2 82.64(12) 2_776 .
O9 Ba1 O2 126.21(13) . .
O26 Ba1 O14 126.9(3) . .
O18 Ba1 O14 143.97(18) . .
O19 Ba1 O14 71.4(2) . .
O11 Ba1 O14 73.31(13) . .
O2 Ba1 O14 64.12(14) 2_776 .
O9 Ba1 O14 129.33(13) . .
O2 Ba1 O14 63.25(13) . .
O26 Ba1 C6 64.1(4) . .
O18 Ba1 C6 19.3(4) . .
O19 Ba1 C6 125.4(4) . .
O11 Ba1 C6 96.1(5) . .
O2 Ba1 C6 118.2(4) 2_776 .
O9 Ba1 C6 61.1(5) . .
O2 Ba1 C6 100.0(4) . .
O14 Ba1 C6 163.2(4) . .
O26 Ba1 V10 115.4(3) . .
O18 Ba1 V10 78.91(16) . .
O19 Ba1 V10 133.95(18) . .
O11 Ba1 V10 29.78(9) . .
O2 Ba1 V10 106.31(9) 2_776 .
O9 Ba1 V10 146.61(10) . .
O2 Ba1 V10 26.13(8) . .
O14 Ba1 V10 66.30(9) . .
C6 Ba1 V10 97.9(4) . .
O26 Ba1 Ba1 179.3(2) . 2_776
O18 Ba1 Ba1 103.56(15) . 2_776
O19 Ba1 Ba1 103.35(16) . 2_776
O11 Ba1 Ba1 92.67(9) . 2_776
O2 Ba1 Ba1 42.20(8) 2_776 2_776
O9 Ba1 Ba1 99.04(10) . 2_776
O2 Ba1 Ba1 40.44(8) . 2_776
O14 Ba1 Ba1 53.82(12) . 2_776
C6 Ba1 Ba1 115.3(3) . 2_776
V10 Ba1 Ba1 64.88(3) . 2_776
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 N1 1.301(16) .
C1 O18 1.428(15) .
C2 N1 1.468(17) .
C3 N1 1.48(2) .
C4 N1A 1.51(4) .
C5 N1A 1.44(4) .
C6 O18 1.26(3) .
C6 N1A 1.32(3) .
C6 Ba1 3.42(2) .
C8 N2 1.52(3) .
C9 N2 1.44(2) .
N2 C7 1.384(19) .
C10 N2A 1.45(2) .
C11 N2A 1.46(2) .
N2A C7 1.418(15) .
C7 O19 1.217(11) .
C12 O26 1.253(15) .
C12 N5 1.408(15) .
C12A O26 1.36(2) .
C12A N5 1.59(3) .
C13 O14 1.243(8) .
C13 N4 1.315(9) .
C14 N4 1.475(9) .
C15 N4 1.456(9) .
C16 N5 1.41(2) .
C17 N5 1.356(18) .
O2 V10 1.640(4) .
O2 Ba1 2.783(4) 2_776
O2 Ba1 2.882(4) .
O3 V5 2.041(4) 2_876
O3 V4 2.115(4) .
O3 V10 2.142(4) .
O4 V5 1.875(4) .
O4 V4 1.987(4) .
O4 V10 1.991(4) .
O5 V10 1.725(4) .
O5 V6 1.983(4) .
O6 V5 2.111(4) 2_876
O6 V5 2.113(4) .
O6 V10 2.224(4) .
O6 V4 2.301(4) 2_876
O6 V6 2.355(4) .
O6 V3 2.366(4) .
O7 V5 1.688(4) .
O7 V6 2.060(4) .
O8 V5 1.680(4) 2_876
O8 V3 2.074(5) .
O9 V4 1.625(4) 2_776
O9 Ba1 2.797(4) .
O10 V4 1.747(4) 2_876
O10 V3 1.951(4) .
O11 V10 1.847(4) .
O11 V3 1.850(4) .
O11 Ba1 2.737(4) .
O12 V6 1.608(5) .
O13 V6 1.798(5) .
O13 V4 1.858(5) 2_876
O14 Ba1 2.911(5) .
O15 V3 1.804(5) .
O15 V6 1.847(5) .
O16 V3 1.610(4) .
O18 Ba1 2.686(7) .
O19 Ba1 2.698(6) .
O26 Ba1 2.632(6) .
V3 V6 3.0892(17) .
V3 V10 3.0906(16) .
V3 V5 3.114(2) 2_876
V4 O9 1.625(4) 2_776
V4 O10 1.747(4) 2_876
V4 O13 1.858(5) 2_876
V4 O6 2.301(4) 2_876
V4 V6 3.090(2) 2_876
V4 V5 3.1161(17) .
V5 O8 1.680(4) 2_876
V5 O3 2.041(4) 2_876
V5 O6 2.111(4) 2_876
V5 V10 3.0850(16) .
V5 V6 3.093(2) .
V5 V3 3.114(2) 2_876
V6 V4 3.0901(19) 2_876
V6 V10 3.1078(16) .
V10 Ba1 3.6258(15) .
Ba1 O2 2.783(4) 2_776
Ba1 Ba1 4.2553(16) 2_776
